Properties of Stabilized Peat by Soil-Cement Column ... - Ejge.com
Vol. 13, Bund. J 2 Deep soil stabilisation technique is often an economically attractive alternative to removal of deep peat or use as deep foundation. The essential feature of deep soil stabilisation is that columns of stabilised material are formed by mixing the soil in place with a ‘binder’ and the interaction of the binder with the soft soil leads to a material which has better engineering properties than the original soil (Hebib and Farrell, 2003). This method is often applied on many geotechnical and foundation applications such as the stabilisation of deep excavations or high embankments, the reduction of settlement or the increase of soil strength for building foundation, the slope stability, the tunnel support, the water retention etc. The strength of soil-cement mixture (the most common binder that is used in DMM) is influenced from many parameters like physicochemical properties of the soil, geological and hydro-geological conditions of the area, the properties and the quality of the used binder or the additive, the mixing method and consequently the mechanical equipment, the curing conditions (Porbaha, 2000). Because of the aforementioned parameters, a significant deviation between the laboratory measurements of strength of soil-cement specimens and the corresponding one taken from in situ is usually observed. The design philosophy for deep stabilisation is to produce a stabilised soil that mechanically interacts with the surrounding unstabilised soil. The applied load is partly carried by the columns and partly by the unstabilised soil between the columns. Therefore, a too stiffly stabilised material is not necessarily the best solution since such a material will behave like a pile (EuroSoilStab, 2002) A study was carried by Wong et al. (2008) found that, the unconfined compressive strength gain of the stabilised peat specimen was only significant after a minimal dosage of 250 kg m -3 binder with 75% cement and 25% slag in composition was added. At the dosage and composition of the binder, its unconfined compressive strength reached 142.5 kPa and with the dosage of binder increased to 300 kg m -3 , the stabilised soil specimen yield the higher unconfined compressive strength of 178.6 kPa as compared to those of other compositions and dosages of the stabilised soil specimens. The high dosage of the binders and siliceous sand required to stabilise the peat can be explained by the fact that the soil has a very low amount of solid particles to be stabilised and hence, more cement, slag and siliceous sand need to be added to the soil to form a sustainable load bearing stabilised soil. Huat et al. (2005) to examine the effect of cement on the unconfined compressive strength of the peat soil sample, namely to examine the effect of cement content and curing period, as well as the influence of organic content on the unconfined compressive strength of the peat soil samples and revealed that increasing the cement content increases the unconfined compressive of the soils samples. Similarly higher strength is obtained from samples that have been cured for 28 days compared with the 3, 7, 14- days cured samples. Bergado et al. (1996) found that pozzolanic reaction can continue for months or even years after mixing, resulting in the increase in strength of cement stabilised clay with the increase in curing time. Objectives of this study were to stabilise peat soil in field by column technique with various types of binder and to observe effect on mechanical strength and microstructure of peat after stabilisation. METHODS AND MATERIALS Soil Characterization The research was conducted from January 2008 to August 2008. The test site was Klang, Peninsular, Malaysia which is located 35 Km North West of Kuala Lumpur city. Trial pits were excavated to a depth of 1 m below the ground surface in order to obtain both undisturbed and disturbed soil samples below the ground water table. Close examination of each trial pit indicated that the ground water table was about 0.3 meter from the ground surface. This showed that the peat had a very high water holding capacity. Visual observation on the peat soil indicated that the soil was dark brown in colour. When the soil was extruded on squeezing (passing between fingers), it could be
Vol. 13, Bund. J 3 observed that the soil was somewhat pasty with muddy water squeezed out, and the plant structure was not easily identified. Table 1 show physical properties of the soils are as follows: Table 1: Physical properties of Klang peat (Hashim and Islam, 2008) Cement A Portland cement particle is a heterogeneous substance, containing minute tri- calcium silicate (C 3 S) dicalicum (C 2 S), tricalcium (C 3 A), and solid solution described as tetra calcium alumino-ferrite (C 4 A). When the pore water of the soil encounters with cement, hydration of the cement occurs rapidly and the major hydration (primary cementitous) produces hydrated calcium silicates (C 2 SH x , C 4 AH x ), and hydrated lime Ca(OH) 2 (Bergado et. al, 1996). In this study we used two types Malaysian local made cement such as YTL cement and Lafarge brand Mascrete cement. Bentonite Bentonite is an absorbent aluminum phyllosilicate which in general terms are impure clay consisting mostly of montmorillonite. Two types exist: swelling bentonite which is also called sodium bentonite and non-swelling bentonite or calcium. It is formed from weathering of volcanic ash, most often in the presence of water. Bentonite expands when wet – sodium bentonite can absorb several hundred percent of its dry weight in water. It is commonly used in drilling fluids, to make slurry walls, and to form impermeable barriers (i.e., plug old wells, as a liner at the base of landfills to prevent migration of leeches eating into the soil). Sand Sand plays a vital role in enhancing the bond in cementation reactions of soil mixing. It is found that grain size distribution provides a satisfactory skeleton, and the voids are filled with fine-sand, giving a compact and high load-bearing capacity. The type of sand used in the laboratory was from Kuala Selangor, Selangor in Malaysia. Calcium chloride (CaCl 2 ) Dehydrate Calcium chloride (CaCl 2 .2H 2 O) has been used as admixture in this experiment. Minimum assay content of this substance was 74%. Maximum impurities were free alkali Iron (Fe) .005% and Magnesium and alkalies (sulphate) 0.5%.